This is an open access article published under a Creative Commons Attribution (CC-BY) License, which permits unrestricted use, distribution and reproduction in any medium, provided the author and source are cited.
Hierarchical Self-Assembly of Cellulose Nanocrystals in a Conﬁned Geometry Richard M. Parker,† Bruno Frka-Petesic,† Giulia Guidetti, Gen Kamita, Gioele Consani, Chris Abell, and Silvia Vignolini* Department of Chemistry, University of Cambridge, Lensﬁeld Road, Cambridge CB2 1EW, United Kingdom S Supporting Information *
ABSTRACT: Complex hierarchical architectures are ubiquitous in nature. By designing and controlling the interaction between elementary building blocks, nature is able to optimize a large variety of materials with multiple functionalities. Such control is, however, extremely challenging in man-made materials, due to the diﬃculties in controlling their interaction at diﬀerent length scales simultaneously. Here, hierarchical cholesteric architectures are obtained by the self-assembly of cellulose nanocrystals within shrinking, micron-sized aqueous droplets. This conﬁned, spherical geometry drastically aﬀects the colloidal self-assembly process, resulting in concentric ordering within the droplet, as conﬁrmed by simulation. This provides a quantitative tool to study the interactions of cellulose nanocrystals beyond what has been achieved in a planar geometry. Our developed methodology allows us to fabricate truly hierarchical solid-state architectures from the nanometer to the macroscopic scale using a renewable and sustainable biopolymer. KEYWORDS: liquid crystals, microﬂuidics, colloidal self-assembly, cellulose nanocrystals, hierarchical architecture
Exploitation of cellulose has existed since the beginning of civilization, from clothes and paper to use as a construction material,17 yet over the last two decades, it has attracted a growing interest due to its abundance and versatility when processed on the nanoscale in the form of cellulose nanocrystals.18 By strong acid hydrolysis, CNC can be extracted from a variety of natural sources, producing stable aqueous suspensions that exhibit cholesteric liquid-crystalline behavior at higher concentrations. 19 The evaporation of CNC suspensions on a ﬂat substrate can result in the formation of a solid ﬁlm with a periodic chiral structure that can reﬂect visible light.20 Traditionally, the self-assembly of such colloidal liquid-crystal systems has been studied in planar geometries,21−23 oﬀering a large variety of applications, for example, in pressure or temperature sensors.24,25 However, more recently, there has been increasing study into the eﬀects of topological constraints.26 Of particular interest is the spherical geometry, where the curvature imposed, for example, by the interface of an emulsiﬁed droplet leads to frustrated liquid-crystalline self-organization.27 This spherical topology, either as a droplet or as a thin shell of liquid, has been shown to give rise to peculiar phenomena, with potential applications in actuators or lasers.16,28,29
esigning and controlling the interaction of elementary building blocks into complex hierarchical architectures enables nature to optimize a large variety of materials with multiple functionalities.1−3 Within the fascinating variety of designs and materials, helicoidal architectures are a recurring motif in nature,4−8 yet little is known about the natural assembly process.9 Consequently, the ability to fabricate biomimetic replicas is fundamentally important not only to elucidate the design principles that underlie the evolution of complex hierarchical structures in nature but also to inspire the development of materials where their functionalities are encoded in the building blocks that compose them.10−12 However, control across a diversity of length scales ranging from nanometers to several hundreds of microns is extremely challenging in man-made materials.13 Here, inspired by the helicoidal architectures found in the plant cell wall,14 we study the assembly of cholesteric architectures of cellulose nanocrystals (CNCs) conﬁned within monodisperse micron-sized droplets, generated via dropletbased microﬂuidics.15,16 The self-assembly process is monitored with polarized optical microscopy, and the eﬀect of the initial aqueous CNC concentration on the resultant self-assembled architecture is studied. This system not only allows for the localized, quantitative investigation of the complex dynamic interaction of CNCs in suspension but also oﬀers a pathway to obtain highly hierarchical structures in a conﬁned geometry from the nanometer to the macroscopic scale, using a renewable and sustainable polymer. © 2016 American Chemical Society
Received: May 20, 2016 Accepted: August 26, 2016 Published: August 26, 2016 8443
DOI: 10.1021/acsnano.6b03355 ACS Nano 2016, 10, 8443−8449
Figure 1. (a) Phase behavior of CNC suspensions of increasing concentration, as imaged under cross-polarizers, where a clear transition from pure isotropic to anisotropic phase is observed from left to right. (b) Calculated ratio of anisotropic phase present for each concentration investigated in (a) was used to compile the phase diagram (crosses). The speciﬁc concentrations investigated within microdroplets are indicated by the colored circles. (c) Polarization micrograph of the generation of microﬂuidic water-in-oil droplets from a 14.5 wt % suspension of CNCs, as imaged under cross-polarizers (right) and with a ﬁrst-order tint plate (left), illustrating the initial radial assembly.
the ﬂuorophilic substrate rather than at the air−oil interface (Figure S2, Supporting Information). The presence of this oil layer slows the loss of water from the droplets, allowing them to be studied over time scales from hours to days. Microdroplets with a typical diameter of 140 μm were prepared from a series of CNC concentrations across the phase transition, as indicated by the colored circles in Figure 1b. In all cases, the optical anisotropy of the suspension allowed for the ordering of CNC domains to be visualized during droplet formation by polarized optical microscopy, as described in the Experimental Methods. This is exempliﬁed with a 14.5 wt % CNC suspension, as denoted by the red circle in the phase diagram (Figure 1b). Here, the generation of an interface between the two ﬂuids at the neck of the ﬂow focus resulted in an immediate radial ordering of the CNCs within the microdroplet, giving rise to a pronounced Maltese cross-like pattern when imaged under crossed polarizers (Figure 1c; see Video S1 and Video S2). However, this arrangement is rapidly disrupted by chaotic advection induced within the microdroplet by shearing interactions with its surroundings as it travels along the microﬂuidic channel. At such a high concentration, the suspension is highly viscous and is almost entirely in a liquidcrystalline phase. For this reason, the shear experienced by the cholesteric phase inside the droplet induces many topological defects. This droplet consequentially remains trapped in this disordered anisotropic state without any particular reordering of the structure. Upon subsequent removal of water (by diﬀusion into the oil) and corresponding concentration of the conﬁned suspension, this arrangement is preserved (Figure S3, Supporting Information). A similar trend is observed for a lower concentration of 10.9 wt % (blue circle on Figure 1b). Here, despite microdroplets containing both isotropic and anisotropic phases, the relaxation toward a radial geometry was again not signiﬁcantly observed after initial droplet formation (Figure S4, Supporting Information).
The study of the self-assembly of CNCs in a microdroplet enables (i) the reproducible measurement of the cholesteric pitch at concentrations that are inaccessible with traditional pitch diagrams due to kinetic arrest, and (ii) monitoring of the self-assembly process over a few hours, instead of several days or weeks,30 thereby reducing errors induced by desulfation of the CNC.31
RESULTS AND DISCUSSION An aqueous suspension of cellulose nanocrystals (Figure S1, Supporting Information) was prepared as described in the Experimental Methods. To characterize the lyotropic properties of this suspension, it was diluted to give a series of CNC concentrations from 14.5 to 4.7 wt %, and the proportion of anisotropic phase was evaluated at each concentration (Figure 1a). This enabled the construction of a traditional phase diagram, as shown in Figure 1b. This phase diagram allows for determination of the critical values of CNC concentration for this speciﬁc suspension at which the transition from the isotropic to the anisotropic phase occurs. In order to understand the impact of geometrical conﬁnement, it was necessary to study how the initial concentration of the CNC suspension aﬀected self-assembly within a micronscale droplet. Microdroplets were generated in a single step as an aqueous emulsion in hexadecane oil within a polydimethylsiloxane (PDMS) ﬂow-focusing microﬂuidic device, as described in the Experimental Methods. At the ﬂow-focusing junction, the aqueous CNC suspension intersected perpendicularly with ﬂows of hexadecane oil, resulting in segmentation into monodisperse microdroplets (coeﬃcient of variation 18 MΩ·cm−1). Instrumentation. Microdroplets were imaged in transmission using a Vision Research Phantom Miro ex4-M fast camera, attached to an Olympus IX-71 inverted microscope (10−64× objectives). Polarized optical microscopy was performed in transmission with crossed polarizers. In order to indicate CNC orientation, a sensitive tint plate (Olympus U-TP530) was additionally inserted between the crossed polarizers. SEM images were acquired using a Zeiss Leo Gemini 1530VP system, working at 90° with respect to the electron beam. SEM samples were mounted on aluminum stubs using conductive carbon tape and, to minimize surface charging, sputtered with a 5−10 nm layer of Au/Pd (Emitech K550; I = 55 mA for 10 s). The acceleration voltage used was 2.0 kV, and the working distance was 1−2 mm. Atomic force microscopy (AFM) images were acquired with an Agilent 5500, collected in tapping mode (OTESPA-R3 tip) and at room temperature over a 25 μm2 area. AFM samples were prepared by drop-casting 10 μL of a diluted CNC suspension on to poly(L-lysine)-functionalized mica. After deposition, the samples were rinsed with deionized water and dried under nitrogen ﬂow. Cellulose Nanocrystal Suspension. Cellulose nanocrystals were obtained from the hydrolysis of Whatman No. 1 cellulose ﬁlter paper (30 g) with sulfuric acid (64 wt %, 420 mL) at 64 °C for 30 min, before being quenched using Milli-Q ice and water. Soluble cellulose residues and acid were removed by centrifugation (three steps at 20 000g for 20 min) and dialysis against deionized water (MWCO 12− 14 kDa membrane), and a stable suspension of [CNC] = 2.2 wt % was obtained. Conductivity titration against sodium hydroxide indicated [SO42−] = 205 mmol·kg−1 of CNC.36 The suspension was tipsonicated in an ice bath (Fisherbrand Ultrasonic disintegrator 500 W, amplitude 30% max 8200 J·g−1 of CNC) and vacuum-ﬁltered (8.0 μm then 0.8 μm nitrocellulose, Sigma-Aldrich). The suspension was concentrated by heating at 60 °C in a water bath for 12 h, resulting in a 14.5 wt % (∼9.4% v/v) suspension of CNC. The ionic content of this concentrated suspension was deduced from conductometric titration against sodium hydroxide, complemented by pH measurements before and after potassium chloride addition, and corresponds to the following: 36% surface charge loss by CNC partial desulfation ([SO42−] = 131 mmol·kg−1 of CNC) [CNC−] = 19 mM, the release of [SO42−]free = 10.7 mM, [H+]free = 18.7 mM and [H+]total = 40.4 mM. Planar ﬁlms of CNC were prepared by casting 1.0 mL of a 2.0 wt % CNC suspension in a 3.5 cm diameter polystyrene petri dish, before being allowed to evaporate under ambient conditions. Phase Diagram and Pitch Measurement in Capillaries. The initial 14.5 wt % CNC suspension was diluted with deionized water using a high precision scale, vortexed, and transferred to a ﬂat capillary of suﬃciently large inner dimensions to eliminate any conﬁnement eﬀects (1.00 × 10.00 × 50 mm) and sealed with glass plates and nail polish. The self-assembly was observed after 4 days and later after 95 days with no noticeable change of the critical concentrations (Figure S12). The cholesteric pitch in the glass capillaries was then determined using (i) polarized optical microscopy (TPlan Nikon, 20× (NA = 0.30, WD = 30 mm) and 50× (NA = 0.40, WD = 22 mm) objectives, Figure S13, Supporting Information); the pitch was measured as twice the period of the ﬁngerprint pattern, taking either an average over 10 pitch
ASSOCIATED CONTENT S Supporting Information *
The Supporting Information is available free of charge on the ACS Publications website at DOI: 10.1021/acsnano.6b03355. 8447
DOI: 10.1021/acsnano.6b03355 ACS Nano 2016, 10, 8443−8449
(14) Vignolini, S.; Rudall, P. J.; Rowland, A. V.; Reed, A.; Moyroud, E.; Faden, R. B.; Baumberg, J. J.; Glover, B. J.; Steiner, U. Pointillist Structural Color in Pollia Fruit. Proc. Natl. Acad. Sci. U. S. A. 2012, 109, 15712−15715. (15) Theberge, A. B.; Courtois, F.; Schaerli, Y.; Fischlechner, M.; Abell, C.; Hollfelder, F.; Huck, W. T. S. Microdroplets in Microfluidics: An Evolving Platform for Discoveries in Chemistry and Biology. Angew. Chem., Int. Ed. 2010, 49, 5846−5868. (16) Humar, M.; Muševič, I. 3D Microlasers from Self-Assembled Cholesteric Liquid-Crystal Microdroplets. Opt. Express 2010, 18, 26995. (17) Kim, J.-H.; Shim, B. S.; Kim, H. S.; Lee, Y.-J.; Min, S.-K.; Jang, D.; Abas, Z.; Kim, J. Review of Nanocellulose for Sustainable Future Materials. International Journal of Precision Engineering and Manufacturing-Green Technology 2015, 2, 197−213. (18) Eichhorn, S. J.; Dufresne, A.; Aranguren, M.; Marcovich, N. E.; Capadona, J. R.; Rowan, S. J.; Weder, C.; Thielemans, W.; Roman, M.; Renneckar, S.; Gindl, W.; Veigel, S.; Keckes, J.; Yano, H.; Abe, K.; Nogi, M.; Nakagaito, A. N.; Mangalam, A.; Simonsen, J.; Benight, A. S.; Bismarck, A.; Berglund, L. A.; Peijs, T. Review: Current International Research into Cellulose Nanofibres and Nanocomposites. J. Mater. Sci. 2010, 45, 1−33. (19) Revol, J. F.; Bradford, H.; Giasson, J.; Marchessault, R. H.; Gray, D. G. Helicoidal Self-Ordering of Cellulose Microfibrils in Aqueous Suspension. Int. J. Biol. Macromol. 1992, 14, 170−172. (20) Revol, J. F.; Godbout, L.; Gray, D. G. Solid Self-Assembled Films of Cellulose with Chiral Nematic Order and Optically Variable Properties. J. Pulp Pap. Sci. 1998, 24, 146−149. (21) Park, J. H.; Noh, J.; Schütz, C.; Salazar-Alvarez, G.; Scalia, G.; Bergström, L.; Lagerwall, J. P. F. Macroscopic Control of Helix Orientation in Films Dried from Cholesteric Liquid-Crystalline Cellulose Nanocrystal Suspensions. ChemPhysChem 2014, 15, 1477− 1484. (22) Roman, M.; Gray, D. G. Parabolic Focal Conics in SelfAssembled Solid Films of Cellulose Nanocrystals. Langmuir 2005, 21, 5555−5561. (23) Beck, S.; Bouchard, J.; Berry, R. Controlling the Reflection Wavelength of Iridescent Solid Films of Nanocrystalline Cellulose. Biomacromolecules 2011, 12, 167−172. (24) Giese, M.; Blusch, L. K.; Khan, M. K.; Hamad, W. Y.; MacLachlan, M. J. Responsive Mesoporous Photonic Cellulose Films by Supramolecular Cotemplating. Angew. Chem., Int. Ed. 2014, 53, 8880−8884. (25) Kelly, J. A.; Shukaliak, A. M.; Cheung, C. C. Y.; Shopsowitz, K. E.; Hamad, W. Y.; MacLachlan, M. J. Responsive Photonic Hydrogels Based on Nanocrystalline Cellulose. Angew. Chem., Int. Ed. 2013, 52, 8912−8916. (26) Jativa, F.; Schütz, C.; Bergström, L.; Zhang, X.; Wicklein, B. Confined Self-Assembly of Cellulose Nanocrystals in a Shrinking Droplet. Soft Matter 2015, 11, 5374−5380. (27) Noh, J.; Reguengo De Sousa, K.; Lagerwall, J. P. F. Influence of Interface Stabilisers and Surrounding Aqueous Phases on Nematic Liquid Crystal Shells. Soft Matter 2016, 12, 367−372. (28) Noh, J.; Liang, H.-L.; Drevensek-Olenik, I.; Lagerwall, J. P. F. Tuneable Multicoloured Patterns from Photonic Cross-Communication Between Cholesteric Liquid Crystal Droplets. J. Mater. Chem. C 2014, 2, 806−810. (29) Muševič, I. Nematic Colloids, Topology and Photonics. Philos. Trans. R. Soc., A 2013, 371, 20120266. (30) Schütz, C.; Agthe, M.; Fall, A. B.; Gordeyeva, K.; Guccini, V.; Salajkova, M.; Plivelic, T. S.; Lagerwall, J. P. F.; Salazar-Alvarez, G.; Bergström, L. Rod Packing in Chiral Nematic Cellulose Nanocrystal Dispersions Studied by Small-Angle X-Ray Scattering and Laser Diffraction. Langmuir 2015, 31, 6507−6513. (31) Beck, S.; Bouchard, J. Auto-Catalyzed Acidic Desulfation of Cellulose Nanocrystals. Nord. Pulp Pap. Res. J. 2014, 29, 006−014. (32) Sen, D.; Mazumder, S.; Melo, J. S.; Khan, A.; Bhattyacharya, S.; D’Souza, S. F. Evaporation Driven Self-Assembly of a Colloidal
AFM of CNC rods, additional images of cholesteric droplets, evolution pitch diagrams, comparative SEM of cross sections of ﬁlms and microdroplets prepared from the same suspension, comparison of pitch measurements by laser diﬀraction and optical microscopy, droplet size distribution and their drying rate; with supplementary discussions on the evaporation process, phase diagram, pitch diagram, and modeling of the optical behavior of cholesteric droplets (PDF) Video S1 (AVI) Video S2 (AVI)
AUTHOR INFORMATION Corresponding Author
*E-mail: [email protected]
. Author Contributions †
R.M.P. and B.F.-P. contributed equally to this work.
The authors declare no competing ﬁnancial interest. Additional data related to this publication is available at the University of Cambridge data repository (http://dx.doi.org/10. 17863/CAM.1233).
ACKNOWLEDGMENTS This work was supported by a BBSRC David Phillips fellowship [BB/K014617/1], the Isaac Newton Trust Cambridge , and the European Research Council [ERC-2014-STG H2020 639088]. REFERENCES (1) Wegst, U. G. K.; Bai, H.; Saiz, E.; Tomsia, A. P.; Ritchie, R. O. Bioinspired Structural Materials. Nat. Mater. 2015, 14, 23−36. (2) Aizenberg, J.; Fratzl, P. Biological and Biomimetic Materials. Adv. Mater. 2009, 21, 387−388. (3) Ortiz, C.; Boyce, M. C. Bioinspired Structural Materials. Science 2008, 319, 1053−1054. (4) Neville, A. C. Biology of Fibrous Composites; Cambridge University Press, 1993. (5) Aguilar Gutierrez, O. F.; Rey, A. D. Chiral Graded Structures in Biological Plywoods and in the Beetle Cuticle. Colloids Interface Sci. Commun. 2014, 3, 18−22. (6) Sharma, V.; Crne, M.; Park, J. O.; Srinivasarao, M. Structural Origin of Circularly Polarized Iridescence in Jeweled Beetles. Science 2009, 325, 449−451. (7) Wilts, B. D.; Whitney, H. M.; Glover, B. J.; Steiner, U.; Vignolini, S. Natural Helicoidal Structures: Morphology, Self-Assembly and Optical Properties. Mater. Today: Proceedings 2014, 1, 177−185. (8) Vignolini, S.; Moyroud, E.; Glover, B. J.; Steiner, U. Analysing Photonic Structures in Plants. J. R. Soc., Interface 2013, 10, 20130394. (9) Reis, D.; Vian, B. Helicoidal Pattern in Secondary Cell Walls and Possible Role of Xylans in Their Construction. C. R. Biol. 2004, 327, 785−790. (10) Glotzer, S. C. Assembly Engineering: Materials Design for the 21st Century (2013 P.v. Danckwerts Lecture). Chem. Eng. Sci. 2015, 121, 3−9. (11) Pokroy, B.; Kang, S. H.; Mahadevan, L.; Aizenberg, J. SelfOrganization of a Mesoscale Bristle into Ordered, Hierarchical Helical Assemblies. Science 2009, 323, 237−240. (12) Dumanli, A. G.; van der Kooij, H. M.; Kamita, G.; Reisner, E.; Baumberg, J. J.; Steiner, U.; Vignolini, S. Digital Color in Cellulose Nanocrystal Films. ACS Appl. Mater. Interfaces 2014, 6, 12302−12306. (13) Sanchez, C.; Arribart, H.; Guille, M. M. G. Biomimetism and Bioinspiration as Tools for the Design of Innovative Materials and Systems. Nat. Mater. 2005, 4, 277−288. 8448
DOI: 10.1021/acsnano.6b03355 ACS Nano 2016, 10, 8443−8449
ACS Nano Dispersion During Spray Drying: Volume Fraction Dependent Morphological Transition. Langmuir 2009, 25, 6690−6695. (33) Straley, J. P. Theory of Piezoelectricity in Nematic Liquid Crystals, and of the Cholesteric Ordering. Phys. Rev. A: At., Mol., Opt. Phys. 1976, 14, 1835−1841. (34) Honorato-Rios, C.; Kuhnhold, A.; Bruckner, J. R.; Dannert, R.; Schilling, T.; Lagerwall, J. P. F. Equilibrium Liquid Crystal Phase Diagrams and Detection of Kinetic Arrest in Cellulose Nanocrystal Suspensions. Front. Mater. 2016, 3, 21. (35) Cerda, E.; Mahadevan, L. Geometry and Physics of Wrinkling. Phys. Rev. Lett. 2003, 90, 074302. (36) Beck, S.; Methot, M.; Bouchard, J. General Procedure for Determining Cellulose Nanocrystal Sulfate Half-Ester Content by Conductometric Titration. Cellulose 2015, 22, 101−116. (37) Kahn, F. J. Electric-Field-Induced Color Changes and Pitch Dilation in Cholesteric Liquid Crystals. Phys. Rev. Lett. 1970, 24, 209− 212.
DOI: 10.1021/acsnano.6b03355 ACS Nano 2016, 10, 8443−8449